ARTICLES Zhao et al.
because of their unique electroactive properties, self-doping, solution-phase near-IR (NIR) spectra were measured on a Varian Cary
thermal stability, characteristic optical properties, and water 500 spectrometer. Atomic force microscopy (AFM) images were taken
solubility. As a result, SPANs have generated interest in the on a Digital Instruments nanoscope IIIA (using taping mode). Scanning
areas of rechargeable batteries,40,41 light-emitting diode de- electron microscopy (SEM) images were taken on a Philips SEM XL-
30 microscope. TGA data were recorded on a Perkin-Elmer Instruments,
vices,42 junction devices,43 and in the electrochemical control
Pyris Diamond TG/DTA Thermogravimetric/Differential Thermal
of electrolyte acidity and enzyme activity.44
Analyzer, with a heating rate of 5°C/min in air. ζ potential data were
Very recently, we reported the synthesis of a water-soluble recorded on a Zetaplus Analyzer (Zetaplus, Brookhaven, USA).
single-walled carbon nanotube poly(m-aminobenzene sulfonic SWNT-PABS Graft Copolymer. P3-SWNTs (500 mg) were
acid) graft copolymer (SWNT-PABS).10 The SWNTs em- sonicated in 500 mL of dimethylformamide (DMF) for 2 h to give a
ployed in this work were produced by the HiPco method and homogeneous suspension. Oxalyl chloride (20 mL) was added dropwise
are known to possess a relatively small diameter. The SWNT- to the SWNT suspension at 0 °C under N2. The mixture was stirred at
PABS graft copolymer has excellent water solubility and 0 °C for 2 h and then at room temperature for another 2 h. Finally the
exhibits an order of magnitude increase in electrical conductivity temperature was raised to 70 °C, and the mixture was stirred overnight
over neat PABS. This material formulation has found application to remove excess oxalyl chloride. PABS38 (5 g) dissolved in DMF was
added to the SWNT suspension, and the mixture was stirred at 100 °C
as the active electronic component in an ammonia sensor,45 and
for 5 days. After it was cooled to room temperature, the mixture was
its zwitterionic electronic structure and water solubility have
filtered through a 0.2-µm pore-size membrane and washed thoroughly
been exploited in biological studies on the interaction of neurons with DMF, ethyl alcohol, and deionized (DI) water. The black solid
with carbon nanotubes.46 As we show below, SWNT-PABS was collected on the membrane and dried under vacuum overnight (1.6
is the first nanotube-based graft copolymer that has a ground g).
state that is a hybrid of the electronic structures of the isolated SWNT-PEG Graft Copolymer. P3-SWNTs (1.5 g) were soni-
macromolecular components. In this paper, we report the cated in 800 mL of DMF for 2 h to give a homogeneous suspension.
synthesis of two water-soluble SWNT-graft copolymers by The SWNT suspension was reacted with oxalyl chloride (60 mL), using
covalent functionalization of SWNTs with PABS and poly- the same procedure as was used in the preparation of SWNT-PABS.
(ethylene glycol) (PEG) at gram scale; the starting SWNTs were PEG (15 g, from Aldrich, MW ) 600) was added to the SWNT
produced by the electric arc (EA) method and are known to be suspension, and the mixture was stirred at 100 °C for 5 days. After it
was cooled to room temperature, the mixture was filtered through a
of larger diameter than HiPco material.47 The solubility of
0.2-µm pore-size membrane and washed thoroughly with ethyl alcohol
SWNT-PABS and SWNT-PEG graft copolymers is about 5 and DI water. The black solid was collected on the membrane and
mg/mL according to quantitative optical spectroscopy studies. dried under vacuum overnight (1.2 g).
While SWNT-PEG is a simple material in which the electronic Solubility. A 0.1 mg/mL aqueous solution of the SWNT derivative
structure of the SWNT component is unperturbed by function- was prepared by the sonication of 5.0 mg of the material in 50.0 mL
alization, we provide evidence that SWNT-PABS is the first of DI water for 2 h. The resulting homogeneous brown solution was
covalently functionalized material for which an internally doped diluted with DI water to prepare 0.05, 0.02, and 0.01 mg/mL solutions
electronic structure can be demonstrated. The loading of SWNTs for NIR characterization, and the NIR spectra of the SWNT derivative
in the graft copolymers has been investigated by thermogravi- solutions were measured immediately after preparation of the solution.
metric analysis (TGA). The ζ potential of SWNT-PABS has A saturated solution of the SWNT derivative was prepared by the
been measured in order to obtain information on the mechanism sonication of 20 mg of material in 2 mL of DI water for 2 h. The
resulting suspension was allowed to stand overnight at room temper-
ature. The upper layer was carefully removed with a syringe and diluted
Experimental Section with DI water. The diluted upper layer was used for the NIR
spectroscopic estimation of the concentration of material in the saturated
Purified (P3), EA SWNTs were obtained from Carbon Solutions, aqueous solution, and the solubilities of SWNT-COOH, SWNT-
Inc. (www.carbonsolution.com); to denote the presence of the carboxylic PABS, and SWNT-PEG were determined as 0.7, 5.8, and 5.9 mg/
acid functionality, P3-SWNT material is sometimes referred to as mL, respectively. To check this result on the bulk scale, 50 mg of
SWNT-COOH. The P3-SWNT material is specifically tailored for SWNT-PABS was sonicated in 10 mL of water. The concentration
functionalization chemistry, and it contains 6% carboxylic acid groups48 of SWNT-PABS in solution was measured immediately after soni-
and a relative carbonaceous purity of 70-90%.49 All other chemicals cation and again after 2 days standing to give solubility values of 5.2
were purchased from Aldrich and used as received. Mid-IR spectra and 4.8 mg/mL.
were measured on a Nicolet Magna-IR 560 ESP spectrometer. The
Results and Discussion
(39) Roy, B. C.; Gupta, M. D.; Bhoumik, L.; Ray, J. K. Synth. Met. 2002, 130,
27-33. Synthesis. The synthesis of SWNT-PABS and SWNT-PEG
(40) Barbero, C.; Miras, M. C.; Kotz, R.; Haas, O. Synth. Met. 1993, 55, 1539- graft copolymers are illustrated in Scheme 1. The starting EA
(41) Barbero, C.; Miras, M. C.; Schnyder, B.; Haas, O.; Kotz, R. J. Mater. Chem. P3-SWNTs were obtained from Carbon Solutions Inc.; this
1994, 4, 1775-1783. material is terminated with carboxylic acid groups and has a
(42) Ferreira, M.; Rubner, M. F. Macromolecules 1995, 28, 7107-7114.
(43) Narasimhan, M.; Hagler, M.; Cammarata, V.; Thakur, M. Appl. Phys. Lett. relative carbonaceous purity of 70-90%.49 The carboxylic acid
1998, 72, 1063-1065. functionalized material (P3, SWNT-COOH), was reacted with
(44) Yue, J.; Epstein, A. J. Chem. Soc., Chem. Commun. 1992, 1540-1542.
(45) Bekyarova, E.; Davis, M.; Burch, T.; Itkis, M. E.; Zhao, B.; Sunshine, S.; oxalyl chloride to form the acyl chloride intermediate, which
Haddon, R. C. J. Phys. Chem. B 2004, 108, 19717-19720. was reacted with PABS and PEG to form the corresponding
(46) Hu, H.; Ni, Y.; Montana, V.; Haddon, R. C.; Parpura, V. Nano Lett. 2004,
4, 507-511. graft copolymers. Dilute solutions of SWNT-PABS and
(47) Hamon, M. A.; Itkis, M. E.; Niyogi, S.; Alvaraez, T.; Kuper, C.; Menon, SWNT-PEG in water are gray-black, whereas aqueous solu-
M.; Haddon, R. C. J. Am. Chem. Soc. 2001, 123, 11292-11293.
(48) Hu, H.; Bhowmik, P.; Zhao, B.; Hamon, M. A.; Itkis, M. E.; Haddon, R. tions of PABS are purple, and aqueous solutions of PEG are
C. Chem. Phys. Lett. 2001, 345, 25-28. colorless. The graft copolymers are quite stable, can be
(49) Itkis, M. E.; Perea, D.; Niyogi, S.; Rickard, S.; Hamon, M.; Hu, H.; Zhao,
B.; Haddon, R. C. Nano Lett. 2003, 3, 309-314. synthesized on the gram scale, and are candidates for industrial
8198 J. AM. CHEM. SOC. 9 VOL. 127, NO. 22, 2005
Synthesis and Characterization of SWNT Graft Polymers ARTICLES
Scheme 1. Synthesis of SWNT-PABS and SWNT-PEG Graft
Figure 1. Mid-IR spectra (ATR method) of SWNT-COOH (top), SWNT-
PABS (middle), and SWNT-PEG (bottom).
applications, particularly in biological applications requiring
Mid-IR spectra (ATR method) of SWNT-COOH, SWNT-
PABS, and SWNT-PEG are shown in Figure 1. The peaks due
to the carbonyl stretches of these materials show good cor-
respondence to the expected structure of the SWNTs. The
spectrum of the starting material (SWNT-COOH) shows a
signal at 1705 cm-1, which is due to the carbonyl stretch of the
carboxylic acid group.50,51 The spectra of SWNT-PABS and
SWNT-PEG show absorbances at 1649 and 1740 cm-1, which
can be assigned to the carbonyl vibration of the amide and ester,
TGA Measurements and SWNT Loading. In our previous
work, energy-dispersive X-ray spectroscopy (EDS) was used
to study the loading of SWNTs in the SWNT-PABS graft Figure 2. TGA graphs and derivative curves of SWNT samples. The TGA
graphs are labeled with the wt % of metal residue after ramping the sample
copolymer, and we found that the SWNT component constituted to 1000 °C.
about 17 wt % of the graft copolymer.10 In the present study,
we used TGA to analyze the loading of SWNTs in the graft attained in the HiPco SWNT-PABS graft copolymer,10 which
copolymers, but since the decomposition temperature of PABS indicates that more PABS was attached to the HiPco SWNTs.
(420 °C) is close to the combustion temperature of SWNTs, The loading of SWNTs in the graft copolymer presumably
TGA measurements do not provide a clear separation between reflects the concentration of carboxylic acid groups on the
the two components. Figure 2 shows the TGA graphs and the SWNTs and the cleavage of the carbon nanotube bundles. The
derivative curves of SWNT-COOH, SWNT-PABS, and HiPco SWNTs used in our previous work were shortened by
SWNT-PEG. The weight percentage of metal residue is 8.7% HNO3/H2SO4 treatment,52 and this may be responsible for the
for SWNT-COOH, 3.2% for SWNT-PABS, and 6.2% for higher concentration of carboxylic acid functional groups and
SWNT-PEG, whereas neat PABS did not leave a residue. We the higher degree of SWNT debundling.
repeated the measurement for SWNT-PABS because NIR
By use of the determination of the SWNT loading in the graft
spectroscopy cannot be used to check the TGA result (below).
copolymers, it is possible to estimate the fraction of the carbon
On the basis of these measurements, we estimate the loading
atoms in the SWNTs that become functionalized in the copoly-
of SWNTs in SWNT-PABS and SWNT-PEG to be about 30
mers. For example, the molecular weight of PEG used in the
and 71%, respectively. This result is roughly consistent with
the synthetic yield of the products together with the reactivity research is about 600, so the degree of functionality in SW-
of the starting materials (320% for SWNT-PABS and 80% NT-PEG can be calculated as a molar functionality ) (29/
for SWNT-PEG, based on the weight of the SWNT-COOH 600)/(71/12) ) 1%. Thus only about 1% of the carbons in the
starting material) and is also supported by NIR measurement SWNTs are functionalized with PEG; the same calculation gives
on SWNT-PEG that give a SWNT loading of 72% (see below). a degree of functionality in SWNT-PABS of 4%. The concen-
The difference in the loading is probably a result of the low tration of carboxylic acid groups in the SWNT-COOH starting
reactivity of PEG toward SWNT-COCl; the amine functionality material was determined to be 6% by acid-base titration,48 and
on PABS is a superior nucleophile to the alcohol on PEG. The thus a significant fraction of these residues are retain-
loading of SWNTs in the arc SWNT-PABS is higher than that ed in the SWNT-PEG and SWNT-PABS graft copolymers.
(50) Chen, J.; Hamon, M. A.; Hu, H.; Chen, Y.; Rao, A. M.; Eklund, P. C.; (52) Liu, J.; Rinzler, A. G.; Dai, H.; Hafner, J. H.; Bradley, R. K.; Boul, P. J.;
Haddon, R. C. Science 1998, 282, 95-98. Lu, A.; Iverson, T.; Shelimov, K.; Huffman, C. B.; Rodriguez-Macias, F.;
(51) Hamon, M. A.; Chen, J.; Hu, H.; Chen, Y.; Itkis, M. E.; Rao, A. M.; Eklund, Shon, Y.-S.; Lee, T. R.; Colbert, D. T.; Smalley, R. E. Science 1998, 280,
P. C.; Haddon, R. C. AdV. Mater. 1999, 11, 834-840. 1253-1255.
J. AM. CHEM. SOC. 9 VOL. 127, NO. 22, 2005 8199
ARTICLES Zhao et al.
value of the ζ potential of SWNT-PABS is larger than 30mV
over a wide pH range (from 2 to 10), which indicates that it is
very stable in water at a concentration of 0.05 mg/mL. The
aqueous dissolution mechanism of the PABS moiety can be
attributed to the dominance of the electrostatic and steric
repulsion between the functionalized SWNTs over the van der
Waals attraction that leads to coagulation and precipitation.
SWNT-PEG has less charge than SWNT-COOH since the
functionalization converts the carboxylic acid groups into esters,
nevertheless the solubility of SWNT-PEG is very close to that
of SWNT-PABS presumably due to the oxygen-containing
glycol chain which can form hydrogen bonds with the water
molecules and capture cations present in solution. The absolute
Figure 3. ζ potential of aqueous SWNTs samples at a concentration of value of the ζ potential of AP SWNTs is less than 30 mV from
pH 5 to 8 as expected from the inert graphene surface of the
ζ Potential Measurements. The ζ potential provides an pristine SWNTs, and this indicates that the system has insuf-
indicator of the stability of colloidal systems. Measurements of ficient electrostatic repulsion to maintain its stability at a
the ζ potential have already been used to discuss the density of concentration of 0.05 mg/mL.
acidic sites on the surface of multiwalled carbon nanotubes Nevertheless, the behavior of the AP SWNT sample supports
(MWNTs) and the stability of MWNT/water colloidal sys- the idea that electrolytes can preferentially adhere to the carbon
tems.21,53-58 The ζ potential of a series of aqueous SWNT nanotube surface.59 For example, electrophoretic deposition
samples as a function of pH is shown in Figure 3; the absolute experiments showed that SWNTs migrated toward the positive
value of the ζ potential over a wide pH range (2-10) follows electrode in the presence of NaOH but toward the negative
the order: SWNT-PABS > SWNT-COOH > SWNT-PEG electrode when MgCl2 was in solution with the carbon nano-
> as-prepared (AP) SWNTs, which is consistent with the surface tubes.59
charge of these materials. SWNT-PABS contains sulfonic acid AFM and SEM. AFM images (Figure 4) of the graft
and amine groups that exist in zwitterionic form, and thus it copolymers were obtained by drying aqueous solutions on mica
has the highest charge throughout the pH range. The absolute substrates. SWNT-COOH has an average length of 890 nm
Figure 4. AFM images of (a) SWNT-COOH, (b) SWNT-PABS, and (c) SWNT-PEG. The length and diameter distribution of the graft copolymers are
obtained from the AFM images.
8200 J. AM. CHEM. SOC. 9 VOL. 127, NO. 22, 2005
Synthesis and Characterization of SWNT Graft Polymers ARTICLES
Figure 6. Solution phase NIR spectra of SWNT-PABS in water. The
inset is the plot of absorbance versus concentration (mg/mL) for the SWNT-
PABS standard solutions. Slope ) 9.28, R2 ) 0.997.
Figure 7. Solution-phase NIR spectra of SWNT-PEG in water. The inset
is the plot of absorbance vs concentration (mg/mL) for the SWNT-PEG
Figure 5. SEM images of (a) SWNT-PABS and (b) SWNT-PEG. standard solutions. Slope ) 6.87, R2 ) 0.999.
and average diameter of 5.04 nm. The average length of
SWNT-PABS is about 510 nm, with an average diameter of standard solutions (0.1, 0.05, 0.02, and 0.01 mg/mL) were
4.2 nm. A large number of the nanotubes (63%) in the SWNT- prepared to calibrate the solubility of the graft copolymers by
PABS graft copolymer have a length shorter than 500 nm, and measuring the intensity of the absorption at the second pair of
only a small amount of tubes are longer than 1 µm (11%). About singularities in the density of states (DOS) of the semiconducting
82% of the tubes in SWNT-PABS have bundle sizes less than SWNTs (S22, centered at 9750 cm-1, Figures 6 and 7). The S22
6 nm. The average length and diameter of SWNT-PEG is 580 interband transition is characteristic of the SWNTs and has been
and 4.3 nm, respectively. In fact, the PABS and PEG attached used to evaluate the purity of electric arc produced SWNTs.49,62-65
to the surface of SWNTs should increase the effective diameter By measurement of the intensity of the S22 interband transition
of the SWNTs. So the exact bundle size of the SWNTs is likely (9750 cm-1) of saturated solutions, the solubility of SWNT-
to be smaller than the observed values; it is not uncommon for PABS and SWNT-PEG are found to be 5.8 and 5.9 mg/mL,
functionalization reactions to exfoliate the SWNT bundles. respectively. Application of our previous method62,63 to the
SEM images of SWNT-PABS and SWNT-PEG (Figure 5) results obtained for SWNT-COOH, SWNT-PABS, SWNT-
show that the SWNTs dominate the morphology of both of the PEG, and PABS gives aqueous effective extinction coefficients
graft copolymers. The SEM image of SWNT-PABS shows that of 12.8, 7.3, 9.2, and 1.3 L‚g-1‚cm-1 at 9750 cm-1, respectively.
the SWNTs are entrapped in PABS matrix to give a compos- The effective extinction coefficient found for the SWNT-
itelike appearance,10 while the image of SWNT-PEG shows a COOH material in water (191 L‚mol-1‚cm-1) is lower than the
dispersed network of interconnected SWNTs. values we reported for highly purified samples in DMF.62,63
Electronic Spectroscopy, Solubility, and Electronic Struc- Because PEG is optically transparent throughout the Vis-
ture. Solution-phase UV spectroscopy has been used to NIR region and remains electronically inert in the copolymer,
demonstrate a linear relationship between the absorbance and it is straightforward to use the above spectral data to calculate
solution concentration of soluble carbon nanotubes in dichlo- the loading of SWNTs in the SWNT-PEG graft copolymer.
robenzene,60 chloroform,4,9 tetrahydrofuran,8,61 DMF,62,63 and
water.15 However, a quantitative solubility study of function- (53) Esumi, K.; Ishigami, M.; Nakajima, A.; Sawada, K.; Honda, H. Carbon
1996, 34, 279-281.
alized SWNTs in water has not been reported, and we have (54) Miller, S. A.; Young, V. Y.; Martin, C. R. J. Am. Chem. Soc. 2001, 123,
used solution-phase NIR spectroscopy to investigate the solubil- 12335-12342.
(55) Sun, J.; Gao, L.; Li, W. Chem. Mater. 2002, 14, 5169-5172.
ity of SWNT-PABS and SWNT-PEG in water. A series of (56) Kim, B.; Park, H.; Sigmund, W. M. Langmuir 2003, 19, 2525-2527.
J. AM. CHEM. SOC. 9 VOL. 127, NO. 22, 2005 8201
ARTICLES Zhao et al.
Figure 8. NIR spectra of SWNT-PABS copolymer (solid line), SWNT-
COOH (dashed line), PABS (long dash-dotted line) in water at a Figure 9. NIR spectra of mixtures of SWNT-COOH and PABS in water
concentration of 0.02 mg/mL. The short dashed line is a fit of the function at constant total concentration by weight. The spectra are labeled with the
FIT ) K(a(PABS) + b(SWNT-COOH)) to the SWNT-PABS spectrum, volume ratio of SWNT-COOH (0.01 mg/mL) to PABS (0.01 mg/mL).
which gave K ) 1.0, a ) 0.22, and b ) 0.78. The short dash-dotted line The dashed line is the spectrum of SWNT-PABS copolymer (0.01 mg/
is the difference spectrum obtained from the function DIFF ) SWNT- mL).
PABS - FIT.
This is best accomplished by taking the ratio of the effective
extinction coefficients of SWNT-COOH and SWNT-PEG in
the region of the S22 interband transition, to give a SWNT
loading of 9.2/12.8 ) 72% in SWNT-PEG, which is consistent
with the TGA result.
Figure 8 shows the UV/Vis/NIR absorption spectra of PABS,
SWNT-COOH, and SWNT-PABS in aqueous solution at a
concentration of 0.02 mg/mL. The absorbance centered at 17750
cm-1 in the spectrum of PABS has been assigned to the n f
π* band transition,39 whereas the SWNT-COOH spectrum
shows the characteristic S22 interband transition centered at 9750
cm-1. In the low-energy region, there is an obvious transfer of
spectral weight from the region of the S22 SWNT interband
Figure 10. Plot of SWNT-COOH content in the mixture against the areal
region (∼10 000 cm-1) to a part of the spectrum (∼16 500 absorbance of the corresponding spectra (Figure 9). The solid square symbol
cm-1), which is near where the n f π* transition of PABS is the areal integration with spectral cutoff from 7 500 to 35 000 cm-1, the
occurs (17 750 cm-1).39 To understand the electronic properties solid circular symbol is the areal integration with spectral cutoff from 7 750
of SWNT-PABS, we carried out a normalized least-squares to 11 750 cm-1, and the hollow circular symbol is the areal integration
above the baseline with spectral cutoff from 7 750 to 11 750 cm-1 and is
fit of the spectra of neat SWNT-COOH and PABS to the mainly due to the S22 interband transition of the SWNTs.
spectrum of SWNT-PABS (Figure 8). The best fit to the
experimental spectrum of SWNT-PABS was obtained with the the SWNT-COOH and PABS spectra, and this result provides
function FIT ) 0.22 × PABS + 0.78 × SWNT-COOH, and clear evidence for an electronic interaction between the PABS
a difference spectrum was obtained from the relationship DIF and SWNT functionalities in sharp contrast with the behavior
) SWNT-PABS - FIT. The weighting factors resulting from of SWNT-PEG discussed above.
the NIR fit are clearly at variance with our previous estimation To further understand the nature of the electronic interaction
of the SWNT loading of ∼30% in SWNT-PABS from TGA between SWNT and PABS, we separately prepared aqueous
analysis (above). Taken together with the significant deviations solutions of SWNT-COOH and PABS, each at a concentration
exhibited by the difference spectrum, it is apparent that the of 0.01 mg/mL. These standard solutions were used to prepare
SWNT-PABS spectrum is not a simple additive composite of a series of mixed solutions of different composition (Figure 9).
It is clear that the SWNT-COOH component is the strongest
(57) Li, Y.-H.; Wang, S.; Luan, Z.; Ding, J.; Xu, C.; Wu, D. Carbon 2003, 41,
1057-1062. absorber in this spectral region.
(58) Zhao, L.; Gao, L. Colloids Surf., A 2003, 224, 127-134. Figure 10 shows a plot of the areal absorbance between two
(59) Gao, B.; Yue, G. Z.; Qui, Q.; Cheng, Y.; Shimoda, H.; Fleming, L.; Zhou,
O. AdV. Mater. 2001, 23, 1770-1773. spectral cutoffs (7 500-35 000 cm-1, NIR-Vis-UV region and
(60) Bahr, J. L.; Mickelson, E. T.; Bronikowski, M. J.; Smalley, R. E.; Tour, J. 7 750-11 750 cm-1, S22 interband transition of SWNTs), as a
M. Chem. Commun. 2001, 193-194.
(61) Zhou, B.; Lin, Y.; Li, H.; Huang, W.; Connell, J. W.; Allard, L. F.; Sun, function of the relative concentration of the two components
Y. P. J. Phys. Chem. B 2003, 107, 13588-13592. (SWNT-COOH and PABS). While the intensity due to the
(62) Zhao, B.; Itkis, M. E.; Niyogi, S.; Hu, H.; Perea, D.; Haddon, R. C. J.
Nanosci. Nanotech. 2004, 4, 995-1004. nanotube S22 interband transition follows an approximately linear
(63) Zhao, B.; Itkis, M. E.; Niyogi, S.; Hu, H.; Zhang, J.; Haddon, R. C. J. dependence on SWNT concentration, it is apparent that the
Phys. Chem. B 2004, 108, 8136-8141.
(64) Sen, R.; Rickard, S. M.; Itkis, M. E.; Haddon, R. C. Chem. Mater. 2003, spectral weight captured by the other areal absorbances initially
15, 4273-4279. grows very rapidly as the SWNT component is added, before
(65) Hu, H.; Zhao, B.; Itkis, M. E.; Haddon, R. C. J. Phys. Chem. B 2003, 107,
13838-13842. following a more gradual increase. This confirms that there is
8202 J. AM. CHEM. SOC. 9 VOL. 127, NO. 22, 2005
Synthesis and Characterization of SWNT Graft Polymers ARTICLES
an electronic interaction between SWNT-COOH and PABS a fairly uniform length and diameter. On the basis of TGA
that at the very least is changing the nature of the chromophores measurements, we estimate the loading of SWNTs in SWNT-
in the mixture. On the basis of the sensitivity of the electrical PABS and SWNT-PEG to be about 30 and 71%, respectively.
conductivity of SWNT-PABS to environmental gases such as The NIR spectrum of the SWNT-PABS graft copolymer is
ammonia,45 it seems likely that the electronic interaction may not a simple sum of the SWNT and PABS spectra, and we
not be confined to the excited-state behavior and may involve conclude that this is the first nanotube-based graft copolymer
a ground-state charge-transfer process. In this sense, SWNT- that has a ground state that is a hybrid of the electronic structures
PABS represents the first SWNT graft copolymer in which the of the isolated macromolecular components. These graft co-
electronic structure should be regarded as a hybrid of the two polymers are well suited for use in the preparation of composite
components. This result also explains why the NIR spectrum materials,66 in biological research,46 and for the active element
of SWNT-PABS copolymer is not a simple sum of the two of electronic sensors.45
components and does not reflect the amounts of each compo- Acknowledgment. This research was supported by DOD/
nent. DARPA/DMEA under Award No. DMEA90-02-2-0216. Carbon
Conclusion Solutions, Inc., acknowledges a DARPA Phase I SBIR Award
administered by the U.S. Army Aviation and Missile Command
We report the synthesis of SWNT-PABS and SWNT-PEG
(Award No. W31P4Q-04-C-R171) and AFOSR Phase I STTR
graft copolymers from EA SWNTs at the gram scale. On the
Award No. FA9550-04-C-0122.
basis of mid-IR spectroscopy, we conclude that the PABS and
PEG are covalently bonded to the SWNTs via amide and ester JA042924I
functionalities, respectively. The solubility of both copolymers (66) Sen, R.; Zhao, B.; Perea, D. E.; Itkis, M. E.; Hu, H.; Love, J.; Bekyarova,
is about 5 mg/mL in water. These SWNT graft copolymers have E.; Haddon, R. C. Nano Lett. 2004, 4, 459-464.
J. AM. CHEM. SOC. 9 VOL. 127, NO. 22, 2005 8203